The International Journal of Engineering and Science
1.
The International Journal of EngineeringAnd Science (IJES)||Volume|| 1 ||Issue|| 1 ||Pages|| 22-29 ||2012||ISSN: 2319 – 1813 ISBN: 2319 – 1805Evaluation Of Microstructural Paramaters Of The Synthesised Γ- Teo2 Nanocrystals Using Xrd Principles A.Sinthiya Depart ment of Physics, St. Joseph’s College(Autonomous), Trichy -620 002, Tamil Nadu, Ind ia .----------------------------------------------------------Abstract-----------------------------------------------------------------The synthesised γ-TeO2 nanocrystalshave been indexed in orthorhombic system with lattice energy 81.21 eV.Strain is caused by the presence of dislocations. This has possibility to have dislocations in nanoscale has littlesignificance. The X-ray peak profile study provides peak broadening and asymmet ric peak shapes and tounderstand the micro structural parameters for crystallite size and strain. Present work deals with systematicapplication of Hall-Williamson method for crystallite size estimation, and the modified Williamson -Hall p lotand the modified Warren-Averbach methods yielded physically well justified data for particle size anddislocation densities. The reflections {020}{151} and {002} have the same peak breadth and reflections while{120}{101}{200} and {122} have more or less same peak breadth. The successful application of the newprocedures have indicated that even in nanocrystalline particles dislocations are present.Keyword: Lattice energy, M icro structural parameters, Crystal size and strain, Nanocrystalline particlesdislocations.----------------------------------------------------------------------------------------------------------------------------------------Date of Submission: 07, November, 2012 Date of Publication: 10, November 2012--------------------------------------------------------------------------------------------------------------------------------------- I. Introduction The microstructure of nanomaterials and its relation to macroscopic properties is essential for thedevelopment and application of nanomaterials. The structure of TeO 2 -based glasses, are promising materials foruse in optical fibre o r in non-linear optical devices [1]. X-ray diffract ion is a pro mising tool for structuralanalysis of solid or amo rphous materials and approaches such as use of Sherrer equation, integral breadthanalysis, single-line approximat ion, Hall-Williamson method, etc., have been developed for estimation ofcrystallite size. Nu merous experiments have shown that the strain broadening caused by dislocations can bewell described by a special logarith mic series expansion of the Fourier coefficients of Bragg reflect ion peakprofiles. X-ray diffraction peak pro file analysis is used for the characterization of microstructure either in thebulk or in loose powder materials, which is a nondestructive method yielding a series of interestingmicrostructural parameters[4].Present work deals with systematic application of Hall-Williamson method for theestimation of crystallite size and the strain [2] of the synthesised γ-TeO2 nanocrystals. Also incorporation of theclassical methods of Williamson – Hall and Warren –Averbach and the modified Williamson – Hall a ndmodified Warren Averbach methods, for the analysis of particle size and dislocation densities as suggested byUngar[3] have been attempted for γ-TeO2 .II. Experimental Grey color Telluriu m metal was mixed in lime water (10ml) and 16 drops of nitric acid was added toit, and after a day, yellow co lor mineral telluriu m d io xide was obtained at room temperature. After 20 daysgrown crystals were filtered and dried at roo m temperature. Lime water helps to spread the ions evenly.III. Results And Discussion2.1 Powder XRD pattern The powder sample subjected to X-ray diffracto meter within 2θ range of 20-60 at a scan speed of 7˚per minute using a Cu target and Cu-Kα radiation of 0.15406 nm wavelength at a powder rating of 40kV, 40mAusing Brukker D8 diffracto meter. The XRD pattern (Fig. 1a) has been indexed in Table 1 falls in theorthorhombic system whose unit cell parameters are tabulated in Table 2.www.theijes.com The IJES Page 22
2.
Evaluation Of Microstructural Paramaters Of The Synthesised Γ-Teo2 Nanocrystals…A bar diagram is drawn between I/I max and δ, which is shown in Figure- 1b, suggests that for the plane {020} thedensity of atom is high compared to other planes and the least in the plane {15 1}. The density of atoms presentin one plane is calculated fro m the fo rmula δ = , where d is the spacing between each plane, N the numberof atoms in the unit cell and V the volu me of the atom[6].2.2Cohesi ve energ y of i onic crystal γ -TeO2 Cohesive energy of an ionic crystal can be determined used even if the crystal structure is not knownwith the help of Kapustinskii equation [15]. Kapustinskii noted an emp irical increase in the value of Madelingconstant, A, as the coordination number of the ions in the molecular formu la of the compound. Any deviation inthe rule is compensated by a consequent change in the value of Re (the sum of the ionic radii for the cation andanion) and the reduced Madelung constant proposed by Kapustinskii (A div ided by the number of ions in theformula) to calculate the lattice energy of an ionic crystal to a good approximat ion, no matter what its geometrymay be.Kapustinskii collected the reduced Madeulang constant [15], the length conversion factor , and theenergy conversion factor into a simple form o f lattice energy equation U. U={ 287.2 v/( + )}*{1-(0.345/( + ))} kcal/ mo l --- (1)whereZc, Za are the charge on cation and anion, + the ionic radii, and v the number of ions in the molecule.This is calculated to be 81.21eV for γ -TeO2 .2.3 Methods of profile anal ysis For the case that the strain is caused by dislocations, Wilkens computed the mean square strain,assuming that the dislocations are ‘restricted rando mly’ and distributed [7][8][9], < >= ln { } --- (2)where the b is the length of burger vector, ρ the dislocation density, R e the outer cut-off radius and C is thecontrast factor of the dislocations.The contrast factor depends on the relative orientation of line -burgers- anddiffraction vector as well as the elastic constants of the material. Because of the actual dislocation distribution ina sample, it is necessary to average over the screw dislocations, different slip systems and orientation of the slipsystem with respect to the diffraction vector, denoting the average contrast factor by C. Ungar and Tichy [10],showed that for cubic or hexagonal crystals, if the burgers vector distribution is completely random, thedependence of C on the hkl can be exp licit ly calculated.The intensity of the profile is given by the convolutionof size and strain broadening. Thus in Fourier space, it is possible to separate the contributions via the wellknownWarren-Averbachequation . ln A L = ln + ln --- (3)Here A L are the Fourier coefficient computed fro m the profile, and are the coefficients associated withsize broadening and strain broadening respectively. The strain broadening coefficients are computed using therelation = exp (-2π 2 L2 g 2 < >) --- (4)where L is the Fourier length, g is the diffraction vector and < > is the mean square strain. It depends on thediffraction order and vanishes for g 2 =0. Inserting Eq.(4 & 5) in Eq.(3) g ives the modified Warren–Averbach equation [11]. ln A L = ln + L2 b 2 ρ C ln ( ) --- (5)If the strain is caused by dislocations, then the modified Warren -Averbach analysis suggest that ln AL must beplotted against g 2 C instead of g 2 . The successful application of this scheme to γ – TeO2 result a smooth curveis shown in Fig 2.www.theijes.com The IJES Page 23
3.
Evaluation Of Microstructural Paramaters Of The Synthesised Γ-Teo2 Nanocrystals…2.4 Crystallite size estimation According to the Scherrer equation [14], the broadening due to small crystallite size may be expressed as = kλ / t cos θ. --- (6)where is the broadening, solely due to small crystallite size, k a constant whose value depends on particleshape and usually taken as 1.0, t the crystallite size in nanometers, θ the Bragg’s angle and λ the wave length ofincident X-ray beam in n m. It is found for the synthesized γ – TeO2 nanostructured material the calculatedcrystallite size is 170.627 n m for K=1 and crystallite size is 153.565n m for K= 0.9. The Hall-Williamsonmethod is a more accurate method than Scherrer equation for crystallite s ize estimation of powder samples inview of the ability of the former approach to measure pure breadth of the diffraction peaks i.e., that solely due tosmaller crystallite size [2] The total peak broadening is given by cos θ = + η sin θ ---(7)where η is the strain distribution. Fig. 3 shows a plot of Brcosθ versus sinθ with the linear fit yields the slope η= 0.58065 for the target, with the wavelength of the incident X-ray beam used in 0.154 n m. Fo llo wing this, theevaluated crystallite size calculated fro m the intercept is 53.18n m for K=1 and t =47.865n m for K = 0.9.Thepeak breadths of the {020}{101}{120}{200}{002}{122} and {151} reflections, scaled in terms of cosΘ∆θ,where Θ and ∆θ are the Bragg angle and half of the FWHM, respectively are shown in Figure 4 with averagecontrast factors according to modified Williamson Hall p lot resulting a slope 0.06487, obtained from the linearfit. The reflections {020}{151} and {002} have the same peak breadth and the reflections {120}{101}{200}and {122} have more or less same peak breadth. This conforms that the peak profiles has peak broadening andasymmetric peak shapes.2.5 Grain size and dislocation densities Irrespective of diffract ion order, for size broadening and dependence on strain broadening, Williamsonand Hall suggested that the FWHM of diffract ion peak profiles can be written as the sum of the two broadeningeffects [12].It is expressed as ∆K = 0.9/D + ∆KD --- (8) Dwhere ∆K is the strain contribution to peak broadening and D is the average grain size or particle size. Here K=2 sinθ/λ, ∆K = 2 cosθ ∆θ/λ,( θ, ∆θ, and λ are the diffraction angle, half of the FWHM of the diffract ion peak andthe wavelength of X-rays, respectively) and g = K at the exact Bragg position. In the conventional Williamson –Hall p lot, it is assumed that ∆KD is either a linear or quadratic function of K [12]. It is exp ressed as ∆K = 0.9/D + (πAb 2 /2)½ ρ½ (KC½) + (πAb 2 /2) Q½ (K2 C) --- (9)where A and A are the parameters determined by the effective outer cutoff radius of dislocations, b the burgervector of dislocations, C the contrast factor, ρ the dislocation density and Q correlation factor. Eq. (9) showsthat if dislocations are the source of strain in a crystal the proper scaling factor of the breadths (or FWHM) ofthe peak profiles is (KC½) instead of merely K. The FWHM according to conventional Williamson- Hall p lot isshown in Fig 5. The unsymmetric FWHM fo llo w an apparently unsystematic behaviour as a funct ion ofdiffraction vector K (or g). Plotting the same data of FWHM according to the modified Williamson -Hall p lot ,a smooth curve is obtained as expected from Eq.(2) and it is shown in Fig.6The average contrast factorscorresponding to the most common type of edge and screw dislocations in f.c.c and b.c.c crystals were evaluatedas a function of the elastic constants of crystals in a wide range of the elastic anisotropy, A i [ where A i =2C44 /(C11 – C12 ) and Cij are the elastic constants] in the range of 7.2405. C or q = a{1-exp (-A i /b)} + c A i + d --- (10)where the parameters a,b,c and d are fitted to the calculation. The C factors were averaged by assuming that allslip systems permitted in given crystal are equally populated , and that edge and the screw dislocations arepresent with equal probability. The contrast factors were calculated using the following elastic constants for γ-TeO2 C11 = 29.6 GPa, C12 = 21.7 GPa and C44 = 28.6 [13].The average C factor used in the present evaluationis listed in Table 3. The insertion at K = 0 of the curve in Fig. 6 fitted by the standard least square methodprovides a particle size to be D =12.6275 n m.2.6 Scatter matri x To account the grain size of the sample the study on the peak profile is important. The peak profiles ofthe observed reflections of the specimen, in the form of scatter matrix are shown in Figure 7. It is thetopographical view to study the relation between the intensities and their corresponding ∆K. It is observed thatwww.theijes.com The IJES Page 24
4.
Evaluation Of Microstructural Paramaters Of The Synthesised Γ-Teo2 Nanocrystals…except {151} reflection all other reflections are confined, the correspond ing intensities are normalized to andcentered around the maxima of the profiles. The FWHM of {101} and {120} reflections are identical within theexperimental error. Similarly the FWHM of {020} and {151} reflections are identical.IV. Conclusions Though every method has its advantages and disadvantages, yet they are independent to determine setof quantities/parameters. It is always useful to make use of all possibilities of evaluation thereby enhancing theaccuracy of the results as well as identifying better procedure. The system has been indexed analytically withreference to[13], in orthorhombic system yields lattice energy as 81.21 eV. For the plane {020} the density ofatom is high compared to other planes with the least in{151}. Strain is caused by the presence of dislocations.This has possibility to have dislocations in nanoscale has little significance.The perfect applicability of modifiedWilliamson-Hall plot indicates that in the nanocrystalline γ-TeO2 , strain is caused by the presence ofdislocations. This has to be considered as a clear answer to the question raised in the debate about the possibilityto have dislocations in nanoscale.Fro m the conventional Williamson Hall plot the calculated η = 0.58065 fro mthe slope is very close to the both theoretical η value and the cf.[13]. Thus in the sequence of length scales, it isestablished that grain size is less than crystallite size. The crystallite size is certainly the smallest length scalein microstructure, which is not directly related to dislocation densities or distances between dislocation. Table 4summarises the calculated grain size and crystallite size of γ-TeO2 .Fro m the conventional Williamson Hall p lot,the reflections {020}{151} and {002} have the same peak breadth and the reflec tions while {120}{101}{200}and {122} have more or less same peak breadth. The peak profile has peak broadening and asymmetric peakshapes and this value provides the micro structural parameters for crystallite size and strain.Fro m the modifiedWarren-Averbach analysis, including the contrast factor we got the smooth curve and thus it conforms that thestrain is caused by dislocations.V. Acknowledgements We are thankful to Sastra university, Tanjore, Tamil Nadu, India for the Powder XRD data collection ,and to our Institution for providing the opportunity to carry out the work.List of symbolsγ Gammaγ-TeO2 Meta stable form of Telluriu m Dio xideeV Electron voltml milli literXRD X-ray diffractionCu Copper targetKα Radiat ion line due to energetic K-electronsnm Nano meterkV Kilo voltmAM illi A mpereθTetad Inter planar distanceÅ Angstrom Un itI IntensityImax Maximu m intensityδ Density of atoms in one planeg/cm⁻1 Grams per centimeter inverseρ Density of the unit cellN Nu mber of ato ms in unit cellhkl miller indicesln Lograthemic expansioneq. EquationFWHM Full width half maximu mf.c.c Face centered cubic crystalsb.c.c Base centered cubic crystalsGPa Giga Pascalη Etawww.theijes.com The IJES Page 25
5.
Evaluation Of Microstructural Paramaters Of The Synthesised Γ-Teo2 Nanocrystals… Reference [1]. Vogel .E.M.; Weber .M.J.;Krol.D.M .;Phys. Chem. Glasses, 1991, 32,pp 231. [2]. Rehani et al., Crystallite size estimation by XRD principles, Indian J. Pure&Appl.Phys., Feb2006 , 44,pp 157-161. [3]. T.Ungar, Strain broadening caus ed by dislocations, Copyright (C) JCPDS - International center for diffraction data 1997. [4]. Michael B. Kerber et al., Rev.Adv.Mater.Sci. 2005, 10,pp 427-433. [5]. T.Ungar, Material Science and Engineering ,2001 , A309-310,pp 14-22. [6]. M.A.Wahab,Solid State Physics, Second edition (2010), Narosa publishing House, New Delhi, pp 36. [7]. M.Wilkens et al.,Phys.Stat.Sol.,1970, A2, pp 359. [8]. M.Wilkens, In: Fundamental Aspects of Dislocation theory, Vol II, ed. By J.A Simmons,R. de lt and R.Bu llough [Nat. Bu r. Stand. (US) Spec. Publ. No. 317, Washington D.C., 1970], pp. 1195. [9]. M.Wilkens et al.,Phys. Stat.Sol. , 1987, A 104, ppK1.[10]. T.Ungarand G. Tichy et al., Phys.Stat.Sol.,1999, (a) 171,pp 425.[11]. T.Ungar and A.Borbely et al., Appl. Phys. Lett..1996, 69,pp3173.[12]. G.K. W illiamson and W.H. Hall, Acta metal. 1953, 1, pp 22.[13]. J.C. Champarnaud-Mesjard ,J.of Physical and chemistry of solids, 2000, 61, pp 1499-1507.[14]. Scherrer P, Math Phys K,1981, 1 , pp 98.[15]. M.A.Wahab,Solid State Physics, Second edition, Narosa publishing House, New Delhi, 2010;pp 66 www.theijes.com The IJES Page 26
6.
Evaluation Of Microstructural Paramaters Of The Synthesised Γ-Teo2 Nanocrystals…www.theijes.com The IJES Page 27
7.
Evaluation Of Microstructural Paramaters Of The Synthesised Γ-Teo2 Nanocrystals…www.theijes.com The IJES Page 28
8.
Evaluation Of Microstructural Paramaters Of The Synthesised Γ-Teo2 Nanocrystals…www.theijes.com The IJES Page 29
Be the first to comment